Journal of Nuclear Materials 396 (2010) 176–180
Contents lists available at ScienceDirect
Journal of Nuclear Materials journal homepage: www.elsevier.com/locate/jnucmat
Carbon ﬁlm growth and hydrogenic retention of tungsten exposed to carbon-seeded high density deuterium plasmas G.M. Wright a,*, R.S. Al a, E. Alves b, L.C. Alves b, N.P. Barradas b, A.W. Kleyn a,c, N.J. Lopes Cardozo a,d, H.J. van der Meiden a, V. Philipps e, G.J. van Rooij a, A.E. Shumack a, W.A.J. Vijvers a, J. Westerhout a, E. Zoethout a, J. Rapp a,e a
FOM-Institute for Plasma Physics Rijnhuizen, EURATOM-FOM, A Member of the Trilateral Euregio Cluster, Nieuwegein, The Netherlands Instituto Tecnológico e Nuclear, Sacavém, Portugal Leiden Institute for Chemistry, Leiden University, Leiden, The Netherlands d Eindhoven University of Technology, Eindhoven, The Netherlands e Institut für Plasmaphysik, FZ Jülich, Association EURATOM, Jülich, Germany b c
a r t i c l e
i n f o
Article history: Received 12 August 2009 Accepted 2 November 2009
a b s t r a c t Tungsten (W) targets have been exposed to high density (ne 6 4 1019 m 3), low temperature (Te 6 3 eV) CH4-seeded deuterium (D) plasma in Pilot-PSI. The surface temperature of the target was 1220 K at the center and decreased radially to 650 K at the edges. Carbon ﬁlm growth was found to only occur in regions where there was a clear CII emission line, corresponding to regions in the plasma with Te P 2 eV. The maximum ﬁlm thickness was 2.1 lm after a plasma exposure time of 120 s. 3He nuclear reaction (NRA) analysis and thermal desorption spectroscopy (TDS) determine that the presence of a thin carbon ﬁlm dominates the hydrogenic retention properties of the W substrate. Thermal desorption spectroscopy analysis shows retention increasing roughly linearly with incident plasma ﬂuence. NRA measures a C/D ratio of 0.002 in these ﬁlms deposited at high surface temperatures. Ó 2009 Elsevier B.V. All rights reserved.
1. Introduction The tungsten–carbon (W–C) system is of high relevance to ITER since these are the materials used in the current design of the ITER divertor. When dealing with mixed-materials, one has to consider both the physics and the chemistry between the two materials. Of particular concern in this system is the formation of tungsten carbides (i.e. WC, W2C) at elevated temperatures and carbon ﬁlm growth on the tungsten substrate. The formation of tungsten carbide has been observed from annealing carbon ﬁlms on tungsten substrates  and from irradiation of tungsten targets at elevated temperatures (TW P 850 K) with carbon-seeded hydrogenic plasmas [2,3]. The latter of these two mechanisms is possible in the ITER divertor since carbon impurities will be eroded, ionized in the plasma and then redistributed to the ﬁrst wall. The formation of tungsten carbide layers is known to increase hydrogenic retention [4,5], decrease diffusion rates , and decrease surface recombination rates  as com-
* Corresponding author. Address: FOM-Institute for Plasma Physics Rijnhuizen, Postbus 1207, 3430 BE Nieuwegein, The Netherlands. Tel.: +31 30 6096830; fax: +31 30 6031204. E-mail address: [email protected]
(G.M. Wright). 0022-3115/$ - see front matter Ó 2009 Elsevier B.V. All rights reserved. doi:10.1016/j.jnucmat.2009.11.002
pared to a pure W surface. Formation of carbon ﬁlms can dominate the retention properties of the tungsten substrate . This investigation focuses on the formation of carbon ﬁlms and any associated carbide formation in a high plasma ﬂux (1024 m 2 s 1) environment and how it impacts the hydrogenic retention of the material. It is critical to examine these processes in a high ﬂux regime since carbon-based components in ITER will be located at the divertor strikepoints; meaning the region of strongest W–C interaction will also be the region of highest plasma ﬂux in ITER. 2. Experiment The plasma exposures of tungsten (W) samples were performed in the linear plasma generator Pilot-PSI . A Thomson scattering system measures plasma parameters 15 mm in front of the target . Typical operation parameters were central electron densities (ne) and temperatures (Te) of (4.0 ± 0.5) 1019 m 3 and 3.0 ± 0.3 eV respectively (Fig. 1). Both ne and Te follow a peaked distribution across the plasma column with an e-folding length of 5.5 ± 0.5 mm. Surface temperatures were measured with a multiwavelength pyrometer that allows for automatic compensation of changing emissivity; an important consideration to maintain consistent temperature measurements for carbon ﬁlms (high emis-
G.M. Wright et al. / Journal of Nuclear Materials 396 (2010) 176–180
sivity) being deposited on a tungsten (low emissivity) substrate. Central surface temperatures during the exposure were measured to be 1200 ± 30 K with a reduction to 650 ± 70 K at the edges of the plasma column (Fig. 1c). The carbon was introduced into the deuterium plasma through a methane pufﬁng ring positioned 150 mm downstream from the plasma source (350 mm upstream from the target). The carbon content of the plasma was monitored with a high resolution spectrometer from 425–435 nm allowing for observation of CII line (426.8 nm), the CH A-X (Gerö) band (429–431.3 nm), and Hc(434.0 nm). It should be noted that in these experiments CH4 was puffed into deuterium plasmas so that any detected deuterium in the analysis originates from the plasma. The spectrometer was focussed at a point 50 mm in front of the target to eliminate any signal contributions from carbon re-erosion from the target surface. The W targets used were 20 mm in diameter and 1 mm thick, 99.97 at.% pure tungsten purchased from Plansee Metals. The targets were mechanically attached to a water-cooled copper heat sink with a molybdenum clamping ring and were electrically grounded for the exposures. No special preparation (i.e. polishing, annealing) of the targets was performed before exposure in PilotPSI. See Table 1 for exposure conditions and nomenclature for each target. The deposited carbon ﬁlms were analyzed by proton microbeam Rutherford backscattering (RBS). The non-Rutherford, enhanced cross section between protons and carbon allow for the deposited carbon to be measured above the strong RBS signal from the high-Z W substrate. X-ray Photoelectric Spectroscopy (XPS)
was used to examine post-exposure surface conditions and check for tungsten carbide formation. The deuterium trapping was investigated using D(3He, p)a Nuclear Reaction Analysis (NRA) and Thermal Desorption Spectroscopy (TDS).
3. Results and discussion Optical emission spectroscopy is used to determine the carbon content of the plasma. The peak signal strengths of the CII-line (426.8 nm), CH band (peak at 430.6 nm), and Hc (434.0 nm) are plotted as a function of radial position in Fig. 2 for CH4 ﬂows of 3 sccm (0.003 slm) and 7 sccm (0.007 slm). One can see that both the methane ﬂow rate and plasma parameters (related through the radial position, see Fig. 1a,b) have a strong inﬂuence on the carbon content of the deuterium plasma. For a CH4 injection rate of 7 sccm, the CII line is not strong in the outer regions of the plasma but only in the central part of the column with Te P 2 eV (Fig. 2). For the 3 sccm injection rate, both the CH-band and CII line are strongly reduced as compared to the 7 sccm case, but the Hc remains constant, indicating that the methane pufﬁng is not affecting the hydrogenic content of the plasma. This is not surprising given the low rate of methane pufﬁng (0.003–0.007 slm) compared to the neutral deuterium injection rate into the plasma source (1.0 slm). Converting these emission proﬁles into plasma carbon concentrations is a highly complex process at the low electron temperatures used in this experiment since photon efﬁciencies no longer follow the standard model . There are experimentally obtained CH photon efﬁciencies  but these are for methane pufﬁng from the surface of the target directly into the plasma column, rather than the pufﬁng ring used to carbon-seed the plasma in this experiment. Nevertheless, since pufﬁng directly into center of the plasma column results in the least amount of injected particles lost before emitting a photon, using these experimentally obtained photon efﬁciencies provides the minimum possible carbon concentrations ((C+ + C0)/D+) of 0.003 and 0.0008 for CH4 puff rates of 7 sccm and 3 sccm respectively. To deﬁne the maximum possible carbon concentration we assume every injected methane atom contributes one carbon atom (or CHX molecule) to the plasma. Under that assumption a comparison of injected gas rates can yield a maximum carbon concentration. The D gas (D2) is injected into the source at a rate of 1.0 slm. Previous work with the cascaded arc source has shown the ionization efﬁciency of the source to be 15% for this gas ﬂow rate , meaning an equivalent D+ ‘‘gas ﬂow rate” of 0.3 slm. Comparing this with the CH4 injection rates of 0.007 slm and 0.003 slm we obtain maximum carbon concentrations of 0.023 and 0.010 respectively. It should be noted that these maximum values are very conservative given we are pufﬁng methane from a ring of diameter 90 mm into a plasma column of diameter < 20 mm. It is likely a signiﬁcant fraction of the injected gas is pumped out of the system without ever penetrating the plasma which would reduce the maximum carbon fraction. However, it can be stated with conﬁdence that the carbon concentrations for plasmas with 7 sccm CH4 injection is in the range 0.003–0.023 and 3 sccm CH4 injection is in the range 0.0008–0.010. Table 1 Carbon seeding conditions and nomenclature for W targets.
Fig. 1. Thomson scattering proﬁles of (a) electron density, (b) electron temperature taken across the plasma column width and (c) surface temperature measurements for a typical plasma exposure.
CH4 puff rate
I – 0–120 VI – 7–10 VII – 7–30 IV – 7–60 VIII – 7–120 IX – 3–120
0 sccm 7 sccm 7 sccm 7 sccm 7 sccm 3 sccm
120 s 10 s 30 s 60 s 120 s 120 s
G.M. Wright et al. / Journal of Nuclear Materials 396 (2010) 176–180
Fig. 2. Radial distribution of CII (426.8 nm), CH (430.6 nm) and Hc (434.0 nm) emission signal for methane pufﬁng rates of (a) 3 sccm and (b) 7 sccm.
Proton RBS results yield detailed measurements of C ﬁlm thicknesses. The micro-beam was focussed to a beam spot diameter of 5 lm and then raster scanned over an analysis spot of 170 170 lm2 allowing for good spatial resolution across a carbon spot only 2.7 mm in diameter (see Fig. 3b). The analysis of the carbon spot from W target VIII – 7–120 shows a well-deﬁned carbon spot centered in the plasma column, indicating that C deposition is occurring in the regions of highest plasma density, electron temperature and surface temperature. This area also corresponds quite closely with the region where the CII emission line is strongest (Fig. 2b). Due to the local nature of the deposition (conﬁned to the plasma column) and the close correspondence with the CII proﬁle, it is inferred that the carbon ﬁlm growth is driven and/or initiated by carbon ions in the plasma as opposed to the large neutral ﬂux of carbon and hydrocarbons also striking the surface. Tungsten carbide formation may play a role in initiating the ﬁlm growth since the highest temperatures, thus the best conditions for carbide formation, are at the center of the ﬁlm growth location. However it should be noted that XPS scans showed no carbide formation at the edges of the carbon spot or in the regions outside the carbon spot. The deposited ﬁlm is too thick for XPS to reach to the W–C interface in the center of the spot. However, it should be noted that, because these targets were exposed in the ‘‘as received” condition, it is possible that oxide layers on the surface (detected by XPS) may have impeded carbide formation. The proton RBS spectra yield an areal concentration of carbon in the analysis spot and this, in combination with ﬁtting of the shape of the spectra, yields C ﬁlm thicknesses. In the spectra, the C peak can clearly be seen over the strong tungsten substrate signal due to the non-Rutherford cross section with proton scattering (Fig. 3a).
Fig. 3. (a) RBS spectra at various locations around carbon ﬁlm on target VIII – 7–120 and (b) measured carbon ﬁlm thicknesses by ﬁtting l-beam proton RBS spectra.
The larger and broader C peaks correspond to thicker C ﬁlms. As the C peak grows, the leading edge of the W component of the spectrum shifts to lower channels/energies, indicating there is no longer any W detectable on the surface. This is conﬁrmed by XPS. The indications from the RBS spectra are that there is no detectable inter-material mixing between the C and W despite the high surface temperatures (1200 K at the center of the spot) and thus highest C diffusion in W and greatest likelihood for tungsten carbide formation. Literature indicates that any intermixing would be under 50 nm in length scale for timescales of 120 s or less . Since the depth resolution of the RBS is 50 nm it is unlikely that any material mixing is detectable over these time or length scales. The C ﬁlm on target VIII – 7–120 was the thickest (Fig. 3b). The C ﬁlm on target IV – 7–60 was also detectable with RBS although the maximum thickness was only 300 nm. On target VII – 7–30 there was visible discolouration at the beam spot indicating the presence of a carbon deposit but there were too few counts for a reliable ﬁt with the RBS. This indicates that there is a small amount of carbon on the beam spot of VII – 7–30 but the ﬁlm thickness was less than the 50 nm depth resolution. However, XPS measurements did not detect any tungsten substrate at the location of the ﬁlm, meaning the ﬁlm was thicker than the probing depth of the XPS (10 nm for a carbon-dominated surface). It is inferred the carbon ﬁlm on VII – 7–30 is 10–50 nm in thickness. For targets VI – 7–10 and IX – 3–120 there was no visible discolouration of the surface and no carbon was detected with RBS either. The C ﬁlm thicknesses are greatest at the center of the plasma column and decrease as the analysis point moves radially outwards (Fig. 3b), again coinciding
G.M. Wright et al. / Journal of Nuclear Materials 396 (2010) 176–180
with the C-II signal. For target IX – 3–120 with the 3 sccm methane puff rate, it is not surprising there is no carbon ﬁlm formation since Fig. 2a shows that there is minimal C-II signal for the 3 sccm puff rate and thus no carbon ions in the plasma to initiate or drive the C ﬁlm growth. Sze et al. have also found a minimum required carbon concentration in the plasma to initiate carbon ﬁlm growth on tungsten . The minimum required carbon content for ﬁlm growth found by Sze et al. was 0.75 at.% at 850 K, however, this minimum decreased with increasing surface temperature. So it is possible for a lower minimum impurity level to be applicable in this study considering surface temperatures and plasma ﬂux densities are higher. However, the minimum required carbon content value in combination with the fact that there was carbon ﬁlm growth for 7 sccm puff rates and not for 3 sccm, indicates that the carbon content of the plasmas in this study are likely much closer to their calculated minimum values than the maximum values. For target VI – 7–10, the lack of detectable carbon indicates either some time delay before ﬁlm growth can be initiated or a very thin ﬁlm undetectable by RBS or by eye. XPS results were inconclusive on this target. The effect of the carbon ﬁlm on overall retention is determined with TDS. W targets were heated to 1273 K at a rate of 1 K/s and the mass 4 (D2) and mass 3 (HD) signals were monitored and calibrated to yield the total amount of retained deuterium. The peak structure changes dramatically between targets VIII – 7–120 and I – 0–120 (Fig. 4a). By comparing the desorption peak structure from VIII – 7–120 to the desorption peak structure from a pure graphite target desorption, it becomes evident that the desorption peaks in target VIII – 7–120 are dominated by the carbon ﬁlm. Integrating the mass 4 and mass 3 signals the total D atoms retained in target VIII – 7–120 (Dretained = 2.0 1016 D atoms) is an order of magnitude greater than in target I – 0–120 (Dretained = 1.6 1015 D atoms) despite the carbon spot only covering 5.7 mm2 of the 200 mm2 exposed area of the tungsten target. The total retention scales roughly linearly with plasma exposure time (a plasma ﬂuence) as shown in Fig. 4b. This is expected for retention dominated by carbon co-deposition since this is an unsaturable retention mechanism. The zero offset in Fig. 4b is indicative of a minimum carbon ﬁlm thickness before retention starts to become dominated by the co-deposition process. The total incident D ﬂuence to the target can be determined through the integration of the bohm ﬂux as determined by the Thomson scattering data (Fig. 1). Retained fractions (Dretained/Dincident) for targets with carbon ﬁlms present is (2 ± 1) 10 6. NRA was used to determine the retention locally, however, due to limited 3He ion energies, the maximum depth range for the NRA measurements was only 3 lm. Measurement spots were taken at the center of the carbon spot, 2 mm off spot and 8 mm off spot. It is important to recognize that at these different locations the surface temperature and plasma ion ﬂuxes are different as well as the carbon content of the plasma. The NRA results clearly show an enhanced retention in the region of the carbon spot (Fig. 5). Retention in the region off the carbon spot is relatively unchanged supporting the results from TDS that the carbon ﬁlm growth is responsible for the overall enhanced retention. Results are also consistent with the observation of no carbon ﬁlm growth with a CH4 injection rate of 3 sccm. The retention from 3 sccm injection rates are equivalent to those observed for exposure times of 10 and 30 s for 7 sccm injection rates where there is no or very little C deposition. The D retention for 2 mm off spot is slightly higher probably due to the lower local surface temperature while still being on the edge of the deposition region. The D retention for 8 mm off spot should not be inﬂuenced by carbon deposition and indicates the range in the natural scatter of retention data from target to target. This scatter has been discussed in more detail in . For the 120 s exposure time the regions of C
Fig. 4. (a) Mass 4 desorption spectrum from clean W, W + C, and pure C and (b) total D retention as a function of plasma exposure time and total incident D ﬂuence; open symbol represents target I – 0–120 (no injected CH4) and closed symbols represent targets VI – 7–10, VII – 7–30, IV – 7–60, and VIII – 7–120 (7 sccm CH4 pufﬁng rate).
Fig. 5. Closed symbols are D retention as measured by NRA as a function of plasma exposure time for various radial positions and CH4 pufﬁng rate of 7 sccm. Open symbols represent target IX – 3–120 (3 sccm CH4 pufﬁng rate).
deposition (i.e. beam center and 2 mm off center) are roughly a factor of 10 higher than D retention in these regions for the 3 sccm injection rate with no C deposition, remaining consistent with the TDS results. NRA can produce depth proﬁles of local D concen-
G.M. Wright et al. / Journal of Nuclear Materials 396 (2010) 176–180
trations. The NRA parameters used for this study yield a depth proﬁle in discrete steps of 1 lm. Since the ﬁlm thickness for target VIII – 7–120 is greater (2 lm) than the discrete step size of the depth proﬁle (1 lm), it is possible to determine the local D concentration within the C ﬁlm and thus determine the D/C ratio. For target VIII – 7–120, the D/C ratio of the ﬁlm at the center location (Tsurf 1200 K) is 0.002 D/C. This low ratio is not unexpected for such high surface temperatures since it is well known that D/C ratios decrease with increasing surface temperatures  and can be < 0.01 D/C for temperatures above 1000 K .
to tungsten targets exposed to plasmas with no carbon seeding. Not only does the carbon ﬁlm enhance retention, it dominates the retention properties of the tungsten targets. This indicates that, while pure tungsten targets have acceptable low hydrogenic retention rates for ITER, if a thick carbon (or any low-Z) ﬁlm is co-deposited on the surface, the retention can become unfavorable, even if those ﬁlms are deposited in a high density, high surface temperature scenario, such as the ITER divertor strikepoint regions.
This work, supported by the European Communities under the contract of the Association EURATOM/FOM, was carried out within the framework of the European Fusion Programme with ﬁnancial support from NWO. The views and opinions expressed herein do not necessarily reﬂect those of the European Commission.
The most obvious observation is the local deposition of carbon ﬁlms on the tungsten substrates. Having the deposition be localized to the center of the plasma column indicates a conﬁnement process was involved and in combination with the close correlation between carbon spot diameter and C-II signal proﬁle, leads to the conclusion that the carbon ﬁlm growth is initiated and/or driven by carbon ions in the plasma and not neutral atoms or molecules. This ﬁlm growth can be rapid (highest measured deposition rate is 17.5 nm/s) in these high plasma density, high surface temperature scenarios, however the resulting ﬁlms have low D/C ratios (0.002 D/C) due to the high surface temperatures during ﬁlm growth. The rapid ﬁlm growth under these conditions could lead to ﬂaking and dust production from very thick deposits in a long pulse or steady-state device. It is also evident that net deposition of carbon is possible on a surface under high ﬂux hydrogenic plasma bombardment even with low (<2%) carbon concentration in the plasma. The growth of C ﬁlms on the surface clearly enhances the hydrogenic retention of the tungsten targets. The enhanced retention is localized to the region of co-deposition and the regions where no ﬁlm was formed have roughly equivalent retention rates
References  J. Luthin, Ch. Linsmeier, J. Nucl. Mater. 290–293 (2001) 121.  F.C. Sze, L. Chousal, R.P. Doerner, S. Luckhardt, J. Nucl. Mater. 266–269 (1999) 1212.  Y. Ueda, T. Shimada, M. Nishikawa, Nucl. Fusion 44 (2004) 62.  V.Kh. Alimov, J. Roth, R.A. Causey, D.A. Komarov, Ch. Linsmeier, A. Wiltner, F. Kost, S. Lindig, J. Nucl. Mater. 375 (2008) 192.  W. Wang, V.Kh. Alimov, B.M.U. Scherzer, J. Roth, J. Nucl. Mater. 241–243 (1997) 1087.  H. Atsumi, T. Tanabe, J. Nucl. Mater. 258–263 (1998) 896–901.  G.J. van Rooij, V.P. Veremiyenko, W.J. Goedheer, et al., Appl. Phys. Lett. 90 (2007) 121501.  H.J. van der Meiden, R.S. Al, et al., Rev. Sci. Instrum. 79 (2008) 013505.  J. Westerhout et al., Appl. Phys. Lett. 95 (2009) 151501.  W.A.J. Vijvers et al., Phys. Plasmas 15 (2008) 093507.  K. Schmid, J. Roth, J. Nucl. Mater. 302 (2002) 96.  G.M. Wright, A.W. Kleyn, E. Alves, et al., J. Nucl. Mater. 390–391 (2009) 610.  V.Kh. Alimov, D.A. Komarov, J. Nucl. Mater. 313–316 (2003) 599.  M. Mayer, V. Philipps, P. Wienhold, H.G. Esser, J. von Seggern, M. Rubel, J. Nucl. Mater. 290–293 (2001) 381.